lithium metal and undergo a reaction. To cover a rough surface, a thicker interlayer may be necessary but it may come along with an increased resistance if the layer becomes too thick.
The differences in the capacity retention of the cells with different interlayers may also be caused by an inhomogeneous interlayer thickness. Although the thickness should not exhibit large lateral differences, even slight differences (e.g. caused by randomly ablated bigger particles) can cause lateral potential distributions across the interface (cf. chapter 2.4) and lead to a locally higher driving force for decomposition.
Further evidence of the protective effect of the interlayer is given by the impedance spectra of the batteries with and without interlayer.
Although the procedure is not optimized, the positive influence of the interlayer on the ASSBs is visible. A more effective protection may be achieved by using a more conformal deposition method, e.g. ALD.
contributions (e.g. wires and current collectors) have a good electronic conductivity and are too small to be resolved. Other contributions, e.g. the lithium anode are large enough to be measured but their time constant so small that they only appear in a frequency range above 106 Hz. The upper frequency limit of the VMP 300 is 7 MHz, therefore these contributions cannot be detected. Other contributions may have similar time constants and cannot be resolved as the respective semicircles overlap, resulting in one larger contribution. For all these reasons, a reasonable data evaluation was performed using three semicircles in the equivalent circuit. The Nyquist plot of a battery with interlayer after 100 cycles has the same shape as the Nyquist plot of the battery without interlayer but the overall resistance of the battery with interlayer is smaller.
Figure 46: Nyquist plot of a battery without anode|electrolyte interlayer after 100 cycles in the charged (blue empty data points) and discharged (black filled data points) state.
From the differences in the impedance spectra of the charged (delithiated cathode) and discharged (lithiated cathode) battery and the values of the capacitances for the three semicircles, it is possible to attribute the semicircles to the different battery components (Figure A 16). The first semicircle at high frequencies is independent from the state of charge (SOC). Therefore, it can be concluded that this semicircle is caused by the solid electrolyte.
This suggestion is supported by the capacitance that was calculated from the CPE, and which 0 1000 2000 3000 4000 5000
0 1000 2000 3000 4000
5000 Discharged Charged
-Im(Z ) / W
Re(Z ) / W
0 1000 2000 3000 4000 5000 Discharged
Re(Z ) / W
is in the range of 10—11 F – 10—10 F, a typical value for the bulk electrolyte (cf. chapter 3.3) and the resistance (denoted as R1) leads to a conductivity of 1.1 ∙ 10—4 S/cm, which is in good agreement with the conductivity values of LPS known from literature , .
Differences in the electrolyte resistance are due to weighing errors during cell fabrication.
Any change of the electrolyte contribution must be caused by the measurement. It can be due to the volume change/densification of the electrolyte during charging/discharging which may differ due to different cell housings or due to reaction with atmosphere that can occur if the housings are not fully gas tight.
The two contributions at lower frequencies depend on the SOC of the battery. They must be attributed to the cathode material. The anode consists of lithium metal and all changes of the resistance during charging and discharging should be small as the conductivity of lithium does not change. The conductivity of the cathode material depends on the state of charge and should therefore lead to an altering contribution to the Nyquist plot. Both impedance contributions at mid to low frequencies have capacitances in the range of 10—6 F, which is typical for the geometric capacitance of an interface. Therefore, these contributions cannot be due to the bulk electrode materials but must be due to both electrolyte|electrode interfaces. It has to be pointed out that due to the large overlapping of these two contributions, fitting of the data is difficult, especially during the first few battery cycles, when these two contributions are not well pronounced yet. For that reason, the values for the second semicircle may be erroneous, as they are influenced by the large third semicircle at low frequencies.
For an assignment of these contribution, a battery with and without interlayer are compared.
Figure 47 depicts the change of the different contributions of the cell resistance in dependence of the charge/discharge cycles.
As discussed above, the discharge capacity of a battery without interlayer decreases drastically during cycling due to the SEI formation at the anode|electrolyte interface and due to the degradation of the electrolyte|cathode interface. Latter effect also occurs in cells with anode|electrolyte interlayer causing a similar capacity fading during long–term cycling. As the cathode side has a more severe impact on the cycling data, it can be assumed that the contribution that shows the strongest changes in the impedance spectrum is caused by the cathode side. Hence, R3 is attributed to the electrolyte|cathode interface. The fact that the
resistance of this component in the lithiated state conforms to the delithiated state, suggests that the volume change during cycling causes a destruction of the composite cathode leading to higher resistances.
Figure 47: Evolution of the resistances of a battery with and without anode|electrolyte interlayer within several charging/discharging cycles of a battery. An impedance measurement was performed after each charging and discharging step.
On the other side, R2 is attributed to the anode|electrolyte interface. In the battery without interlayer, this contribution is also increasing, suggesting that an interface is formed. But the increase of R2 shows a parabolic behavior in the discharged state. This suggests that the
0 50 100
0 500 1000 1500 2000 2500
R1 R2 R3 discharged R1 R2 R3
Resistance / W
0 50 100
0 500 1000 1500 2000 2500
R1 R2 R3 discharged R1 R2 R3
Resistance / W
growth of R2 is limited. It may therefore be due to the formation of a passivating SEI at the anode|electrolyte interface. On the cathode side, the transition metal ions of nickel, cobalt and manganese should prevent a passivation due to the formation of metal atoms. It can therefore be suggested that R2 is due to the anode|electrolyte interface. However, this resistance is bigger in the discharged state of the battery than in the charged state. If lithium is transported from the anode side to the cathode side of the battery during discharge, voids are formed at the lithium|electrolyte interface and these voids increase the interface resistance. During the first 10 cycles, the data is not according to the trend because due to the small contributions R2 and R3, the same equivalent circuit leads to fitting errors.
All resistances of the battery with interlayer do also increase over time. The increase of the electrolyte resistance R1 is bigger than in the case of the battery without interlayer. As the initial values of R1 are similar in all batteries (Appendix I) and differences are not caused by the intrinsic properties of the electrolyte, this behavior may be due to different pressure on the cell housing. Statistically, the increase of R1 is not bigger than for the cells without interlayer. It has to be pointed out that the values of R1 of the battery without interlayer in Figure 47 do slightly deviate from the apparent diameter of the semicircle in Figure 46. The difference is caused from fitting errors caused by high–frequent noise. As the information from frequencies above 7 MHz is lacking, there is no information on possible additional serial resistances.
R2 does increase in the case of a charged battery with interlayer but stays constant in the discharged state. This observation may be due to the fact that the lithium|electrolyte interface is enhanced by the protective layer and the contact is more homogeneous. When the battery is charged, additional lithium is transported to the anode side and causes a volume expansion of the anode, which increases the resistance. When the additional lithium is removed during discharge, the resistance is decreased again and the anode|electrolyte interface is retrieved as before.
The resistance R3 also increases during cycling. Although R3 is also bigger in the discharged state than in the charged state, in the case of an interlayer, they do not seem to converge.
Therefore, the application of an interlayer on the anode side does not only have an influence on the anode|electrolyte interface but also on the cathode side. A detailed study on the reasons still needs to carried out. It may be possible that according to the thermodynamic
discussion in chapter 2.4, the potential drop on the anode side has an influence on the potential drop on the cathode side. A large potential drop across the SEI creates a strong electric field that can cause a decomposition of the electrolyte. The anode|electrolyte interlayer with a negligible electronic conductivity should cause a strong potential drop across the interlayer. In that case the potential drop on the cathode side should be smaller, leading to a less pronounced decomposition. The change of R3 is then only due to the volume change during cycling.
We conclude that the application of P3N5 as interlayer is an effective way to modify the lithium|electrolyte interface. The material does not only protect the electrolyte from decomposition in contact with lithium metal (Figure 34), it also has a positive influence on the capacity retention of full cells. These experiments with P3N5 successfully prove the concept of sacrificial interlayers in ASSBs.